# ISSUES TO ADDRESS... How do atoms assemble into solid structures? How does the density of a material depend on its structure? When do material properties.

## Presentation on theme: "ISSUES TO ADDRESS... How do atoms assemble into solid structures? How does the density of a material depend on its structure? When do material properties."— Presentation transcript:

ISSUES TO ADDRESS... How do atoms assemble into solid structures? How does the density of a material depend on its structure? When do material properties vary with the sample (i.e., part) orientation? 1 CHAPTER 3: Structures of Metals and Ceramics How do the structures of ceramic materials differ from those of metals?

2 Non dense, random packing Dense, regular packing Dense, regular-packed structures tend to have lower energy. ENERGY AND PACKING

3 tend to be densely packed. have several reasons for dense packing: -Typically, only one element is present, so all atomic radii are the same. -Metallic bonding is not directional. -Nearest neighbor distances tend to be small in order to lower bond energy. have the simplest crystal structures. We will look at three such structures... METALLIC CRYSTALS

4 Rare due to poor packing (only Po has this structure) Close-packed directions are cube edges. Coordination # = 6 (# nearest neighbors) (Courtesy P.M. Anderson) SIMPLE CUBIC STRUCTURE (SC) Click on image to animate

5 APF for a simple cubic structure = 0.52 Adapted from Fig. 3.19, Callister 6e. ATOMIC PACKING FACTOR

6 Coordination # = 12 Adapted from Fig. 3.1(a), Callister 6e. (Courtesy P.M. Anderson) Close packed directions are face diagonals. --Note: All atoms are identical; the face-centered atoms are shaded differently only for ease of viewing. FACE CENTERED CUBIC STRUCTURE (FCC) Click on image to animate

7 APF for a body-centered cubic structure = 0.74 Adapted from Fig. 3.1(a), Callister 6e. ATOMIC PACKING FACTOR: FCC

Coordination # = 8 8 Adapted from Fig. 3.2, Callister 6e. (Courtesy P.M. Anderson) Close packed directions are cube diagonals. --Note: All atoms are identical; the center atom is shaded differently only for ease of viewing. BODY CENTERED CUBIC STRUCTURE (BCC) Click on image to animate

9 APF for a body-centered cubic structure = 0.68 Adapted from Fig. 3.2, Callister 6e. ATOMIC PACKING FACTOR: BCC

10 Coordination # = 12 ABAB... Stacking Sequence APF = 0.74 3D Projection 2D Projection Adapted from Fig. 3.3, Callister 6e. HEXAGONAL CLOSE-PACKED STRUCTURE (HCP)

11 Example: Copper Data from Table inside front cover of Callister (see next slide): crystal structure = FCC: 4 atoms/unit cell atomic weight = 63.55 g/mol (1 amu = 1 g/mol) atomic radius R = 0.128 nm (1 nm = 10 cm) -7 THEORETICAL DENSITY, 

12 Adapted from Table, "Charac- teristics of Selected Elements", inside front cover, Callister 6e. Characteristics of Selected Elements at 20C

13 Why? Metals have... close-packing (metallic bonding) large atomic mass Ceramics have... less dense packing (covalent bonding) often lighter elements Polymers have... poor packing (often amorphous) lighter elements (C,H,O) Composites have... intermediate values Data from Table B1, Callister 6e. DENSITIES OF MATERIAL CLASSES

14 Bonding: --Mostly ionic, some covalent. --% ionic character increases with difference in electronegativity. Adapted from Fig. 2.7, Callister 6e. (Fig. 2.7 is adapted from Linus Pauling, The Nature of the Chemical Bond, 3rd edition, Copyright 1939 and 1940, 3rd edition. Copyright 1960 by Cornell University. Large vs small ionic bond character: CERAMIC BONDING

15 Charge Neutrality: --Net charge in the structure should be zero. --General form: Stable structures: --maximize the # of nearest oppositely charged neighbors. Adapted from Fig. 12.1, Callister 6e. IONIC BONDING & STRUCTURE

16 Coordination # increases with Issue: How many anions can you arrange around a cation? Adapted from Table 12.2, Callister 6e. Adapted from Fig. 12.2, Callister 6e. Adapted from Fig. 12.3, Callister 6e. Adapted from Fig. 12.4, Callister 6e. COORDINATION # AND IONIC RADII

17 On the basis of ionic radii, what crystal structure would you predict for FeO? Answer: based on this ratio, --coord # = 6 --structure = NaCl Data from Table 12.3, Callister 6e. EX: PREDICTING STRUCTURE OF FeO

18 Consider CaF 2 : Based on this ratio, coord # = 8 and structure = CsCl. Result: CsCl structure w/only half the cation sites occupied. Only half the cation sites are occupied since #Ca 2+ ions = 1/2 # F - ions. Adapted from Fig. 12.5, Callister 6e. A m X p STRUCTURES

19 Demonstrates "polymorphism" The same atoms can have more than one crystal structure. DEMO: HEATING AND COOLING OF AN IRON WIRE

20 ABCABC... Stacking Sequence 2D Projection FCC Unit Cell FCC STACKING SEQUENCE

21 Compounds: Often have similar close-packed structures. Close-packed directions --along cube edges. Structure of NaCl (Courtesy P.M. Anderson) STRUCTURE OF COMPOUNDS: NaCl Click on image to animate

22 Some engineering applications require single crystals: Crystal properties reveal features of atomic structure. (Courtesy P.M. Anderson) --Ex: Certain crystal planes in quartz fracture more easily than others. --diamond single crystals for abrasives --turbine blades Fig. 8.30(c), Callister 6e. (Fig. 8.30(c) courtesy of Pratt and Whitney). (Courtesy Martin Deakins, GE Superabrasives, Worthington, OH. Used with permission.) CRYSTALS AS BUILDING BLOCKS

23 Most engineering materials are polycrystals. Nb-Hf-W plate with an electron beam weld. Each "grain" is a single crystal. If crystals are randomly oriented, overall component properties are not directional. Crystal sizes typ. range from 1 nm to 2 cm (i.e., from a few to millions of atomic layers). Adapted from Fig. K, color inset pages of Callister 6e. (Fig. K is courtesy of Paul E. Danielson, Teledyne Wah Chang Albany) 1 mm POLYCRYSTALS

24 Single Crystals -Properties vary with direction: anisotropic. -Example: the modulus of elasticity (E) in BCC iron: Polycrystals -Properties may/may not vary with direction. -If grains are randomly oriented: isotropic. (E poly iron = 210 GPa) -If grains are textured, anisotropic. 200  m Data from Table 3.3, Callister 6e. (Source of data is R.W. Hertzberg, Deformation and Fracture Mechanics of Engineering Materials, 3rd ed., John Wiley and Sons, 1989.) Adapted from Fig. 4.12(b), Callister 6e. (Fig. 4.12(b) is courtesy of L.C. Smith and C. Brady, the National Bureau of Standards, Washington, DC [now the National Institute of Standards and Technology, Gaithersburg, MD].) SINGLE VS POLYCRYSTALS

25 Incoming X-rays diffract from crystal planes. Measurement of: Critical angles,  c, for X-rays provide atomic spacing, d. Adapted from Fig. 3.2W, Callister 6e. X-RAYS TO CONFIRM CRYSTAL STRUCTURE

atoms pack in periodic, 3D arrays typical of: 26 Crystalline materials... -metals -many ceramics -some polymers atoms have no periodic packing occurs for: Noncrystalline materials... -complex structures -rapid cooling crystalline SiO 2 noncrystalline SiO 2 "Amorphous" = Noncrystalline Adapted from Fig. 3.18(b), Callister 6e. Adapted from Fig. 3.18(a), Callister 6e. MATERIALS AND PACKING

28 Quartz is crystalline SiO 2 : Basic Unit: Glass is amorphous Amorphous structure occurs by adding impurities (Na +,Mg 2+,Ca 2+, Al 3+ ) Impurities: interfere with formation of crystalline structure. (soda glass) Adapted from Fig. 12.11, Callister, 6e. GLASS STRUCTURE

Atoms may assemble into crystalline or amorphous structures. We can predict the density of a material, provided we know the atomic weight, atomic radius, and crystal geometry (e.g., FCC, BCC, HCP). Material properties generally vary with single crystal orientation (i.e., they are anisotropic), but properties are generally non-directional (i.e., they are isotropic) in polycrystals with randomly oriented grains. 27 SUMMARY

Reading: Core Problems: Self-help Problems: 29 ANNOUNCEMENTS

Download ppt "ISSUES TO ADDRESS... How do atoms assemble into solid structures? How does the density of a material depend on its structure? When do material properties."

Similar presentations